NATIONAL STANDARD OF THE GRINDING BALLS IN CHINA(5)
5. Technical Requirements
5.1 The grinding balls tolerance of the diameter should be accord with Table 1.
5.2 The main chemical composition of each grades should be accord with Table 2.
|Name||Grade||Chemical Composition (%)|
|Alloyed cast iron grinding balls||ZQCr26||2.0-3.3||≤ 1.2||0.3-1.5||>23.0-30.0||0-3.0||0-1.2||0.-1.5||≤1.0||≤0.06|
|Alloyed cast iron grinding balls||ZQCr20||2.0-3.3||≤ 1.2||0.3-1.5||>18.0-23.0||0-3.0||0-1.2||0.-1.5||≤1.0||≤0.06|
|Alloyed cast iron grinding balls||ZQCr15||2.0-3.3||≤ 1.2||0.3-1.5||>14.0-18.0||0-3.0||0-1.2||0.-1.5||≤1.0||≤0.06|
|Alloyed cast iron grinding balls||ZQCr12||2.0-3.3||≤ 1.2||0.3-1.5||>10.0-14.0||0-3.0||0-1.2||0.-1.5||≤1.0||≤0.06|
|Alloyed cast iron grinding balls||ZQCr8||2.1-3.3||≤ 2.2||0.3-1.5||7.0-10.0||0-1.0||0-0.8||–||≤1.0||≤0.06|
|Alloyed cast iron grinding balls||ZQCr5||2.1-3.3||≤ 1.5||0.3-1.5||4.0-6.0||0-1.0||0-0.8||–||≤1.0||≤1.0|
|Alloyed cast iron grinding balls||ZQCr2||2.1-3.6||≤ 1.5||0.3-1.5||1.0-3.0||0-1.0||0-0.8||–||≤1.0||≤1.0|
|Ductile iron grinding balls||ZQQTB||3.2-3.8||2.0-3.5||2.0-3.0||–||–||–||–||≤1.0||≤0.03|
|Ductile iron grinding balls||ZQQTM||3.2-3.8||2.0-3.5||0.5-1.5||–||–||–||–||≤1.0||≤0.03|
5.3 Mechanical Property
5.3.1 The surface hardness should be accord with Table 3
|NAME||GRADE||SURFACE HARDNESS /HRC|
|Alloyed cast iron grinding balls||ZQCr26||≥58|
|Alloyed cast iron grinding balls||ZQCr20||≥58|
|Alloyed cast iron grinding balls||ZQCr15||≥58|
|Alloyed cast iron grinding balls||ZQCr12||≥58|
|Alloyed cast iron grinding balls||ZQCr8||≥48|
|Alloyed cast iron grinding balls||ZQCr5||≥47|
|Alloyed cast iron grinding balls||ZQCr2||≥45|
|Ductile iron grinding balls||ZQQTB||≥50|
|Ductile iron grinding balls||ZQQTM||≥52|
5.3.2 The hardness between the casting head surface to the centre of the balls can not be over 3 degrees. Diameter balls size over dia90mm, the grade is ZQCr2 and the other special situation, the hardness differences negotiate between the contracting parties.
5.3.3 The broken rate of the Grade ZQCr26, ZQCr20, ZQCr15, ZQCr12 grinding balls should be less than or equal to 1%. The other grades, the broken rate should be less than or equal to 2%. The special conditions, the requirements need to negotiate between the contracting parties.
5.3.4 Whether regarding the impact value as the acceptance standard depends on the contracting parties.
5.4 Casting grinding ball does not allow cracks and the defects, like slag, sand hole, shrinkage hole, shrinkage porosity, gas hole, cold separation, etc. Which will affect the using.
5.5 Metallographic Structure
The metallographic structure is the essential quality inspection content in the production process of casting grinding ball. Not as acceptance standard for products. If there is any special need, both parties should agree on it